Silver Coodination Polymers with Flexible Ligands. Syntheses, Crystal Structures, and Effect of the Counteranion and the Solvent on the Structure of Complexes [AgL1X]∞of the Bis(Phenylthio)methane LigandL1with Silver(I) Salts, X = ClO4-, BF4-, CF3COO-, CF3SO3-, CF3CF2CF2COO-, and-OOCCF2CF2COO-
Awaleh, Mohamed Osman; Badia, Antonella; Brisse, François; Crystal Growth & Design 5 (2005) 1897–; doi:10.1021/cg050180u

data_4505210
_publ_section_title
;
 Silver Coodination Polymers with Flexible Ligands. Syntheses, Crystal
 Structures, and Effect of the Counteranion and the Solvent on the
 Structure of Complexes [AgL1X]\\infty of the Bis(Phenylthio)methane
 LigandL1with Silver(I) Salts, X = ClO4-, BF4-, CF3COO-, CF3SO3-,
 CF3CF2CF2COO-, and-OOCCF2CF2COO-
;
_journal_issue                   5
_journal_name_full               'Crystal Growth &amp; Design'
_journal_page_first              1897
_journal_paper_doi               10.1021/cg050180u
_journal_volume                  5
_journal_year                    2005
_chemical_compound_source        'Synthesized by the authors. See text'
_chemical_formula_moiety         'C15 H12 Ag F3 O2 S2'
_chemical_formula_sum            'C15 H12 Ag F3 O2 S2'
_chemical_formula_weight         453.24
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           14
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-P 2ybc'
_symmetry_space_group_name_H-M   'P 1 21/c 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.882(2)
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   4.93730(10)
_cell_length_b                   19.9552(5)
_cell_length_c                   16.2439(4)
_cell_measurement_reflns_used    4619
_cell_measurement_temperature    220(2)
_cell_measurement_theta_max      72.46
_cell_measurement_theta_min      2.72
_cell_volume                     1600.24(6)
_computing_cell_refinement       'SMART (Bruker, 1999)'
_computing_data_collection       'SMART (Bruker, 1999)'
_computing_data_reduction        'SAINT (Bruker, 1999)'
_computing_molecular_graphics    'SHELXTL (Bruker, 1997)'
_computing_publication_material  'UdMX (local program)'
_computing_structure_refinement  'SHELXL97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS97 (Sheldrick, 1997)'
_diffrn_ambient_temperature      220(2)
_diffrn_detector_area_resol_mean 5.5
_diffrn_measured_fraction_theta_full 0.963
_diffrn_measured_fraction_theta_max 0.963
_diffrn_measurement_device_type  'Bruker Smart 2000'
_diffrn_measurement_method       \w
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'X-ray Sealed Tube'
_diffrn_radiation_type           CuK\a
_diffrn_radiation_wavelength     1.54178
_diffrn_reflns_av_R_equivalents  0.048
_diffrn_reflns_av_sigmaI/netI    0.0739
_diffrn_reflns_limit_h_max       4
_diffrn_reflns_limit_h_min       -5
_diffrn_reflns_limit_k_max       24
_diffrn_reflns_limit_k_min       -24
_diffrn_reflns_limit_l_max       16
_diffrn_reflns_limit_l_min       -19
_diffrn_reflns_number            10160
_diffrn_reflns_theta_full        73.10
_diffrn_reflns_theta_max         73.10
_diffrn_reflns_theta_min         3.51
_diffrn_standards_decay_%        -0.98
_diffrn_standards_number         222
_exptl_absorpt_coefficient_mu    12.898
_exptl_absorpt_correction_T_max  0.313
_exptl_absorpt_correction_T_min  0.135
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'Sadabs (Sheldrick,1996)'
_exptl_crystal_colour            Colorless
_exptl_crystal_density_diffrn    1.881
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       block
_exptl_crystal_F_000             896
_exptl_crystal_size_max          0.23
_exptl_crystal_size_mid          0.12
_exptl_crystal_size_min          0.09
_refine_diff_density_max         0.744
_refine_diff_density_min         -0.651
_refine_diff_density_rms         0.128
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   0.986
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     199
_refine_ls_number_reflns         3078
_refine_ls_number_restraints     117
_refine_ls_restrained_S_all      2.417
_refine_ls_R_factor_all          0.0904
_refine_ls_R_factor_gt           0.0577
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0717P)^2^] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1360
_refine_ls_wR_factor_ref         0.1476
_reflns_number_gt                1951
_reflns_number_total             3078
_reflns_threshold_expression     I>2\s(I)
_cod_data_source_file            cg050180usi20050425_041923.cif
_cod_data_source_block           Complex3
_cod_depositor_comments
;
The following automatic conversions were performed:

'_symmetry_cell_setting' value 'Monoclinic' changed to 'monoclinic'
according to /home/saulius/struct/CIF-dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.1 from
2010-06-29.

'_geom_bond_publ_flag' value 'Y' changed to 'y'
according to /home/saulius/struct/CIF-dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.1 from 2010-06-29 (32
times).

'_geom_angle_publ_flag' value 'Y' changed to 'y' according
to /home/saulius/struct/CIF-dictionaries/cif_core.dic dictionary
named 'cif_core.dic' version 2.4.1 from 2010-06-29 (67 times).

Automatic conversion script
Id: cif_fix_values 1715 2011-07-08 13:25:40Z adriana 
;
_cod_original_sg_symbol_H-M      P21/c
_cod_database_code               4505210